#------------------------------------------------------------------------------
#$Date: 2016-03-25 23:02:06 +0200 (Fri, 25 Mar 2016) $
#$Revision: 180023 $
#$URL: svn://www.crystallography.net/cod/cif/7/03/17/7031711.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7031711
loop_
_publ_author_name
'Carrasco, Carlos J.'
'Montilla, Francisco'
'Alvarez, Eleuterio'
'Mealli, Carlo'
'Manca, Gabriele'
'Galindo, Agustín'
_publ_section_title
;
 Experimental and theoretical insights into the
 oxodiperoxomolybdenum-catalysed sulphide oxidation using hydrogen
 peroxide in ionic liquids.
;
_journal_issue                   36
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              13711
_journal_page_last               13730
_journal_paper_doi               10.1039/c4dt01733a
_journal_volume                  43
_journal_year                    2014
_chemical_formula_moiety         'C6 H8 Mo8 N4 O28, 4(C3 H5 N2), 3(H2 O)'
_chemical_formula_sum            'C18 H34 Mo8 N12 O31'
_chemical_formula_weight         1682.09
_chemical_name_systematic
;
  ?
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                93.182(2)
_cell_angle_beta                 117.554(2)
_cell_angle_gamma                101.937(2)
_cell_formula_units_Z            1
_cell_length_a                   10.6258(7)
_cell_length_b                   10.6937(8)
_cell_length_c                   11.2851(8)
_cell_measurement_reflns_used    7363
_cell_measurement_temperature    173(2)
_cell_measurement_theta_max      30.36
_cell_measurement_theta_min      2.60
_cell_volume                     1095.26(14)
_computing_cell_refinement       'Bruker (2006). APEX 2. Version 2.1.'
_computing_data_collection       'Bruker (2006). APEX 2. Version 2.1.'
_computing_data_reduction        'Bruker (2006). APEX 2. Version 2.1.'
_computing_molecular_graphics    'XP, SHELXTL v. 6.14 (Bruker, 2003)'
_computing_publication_material  'XCIF, SHELXTL v. 6.14 (Bruker, 2003)'
_computing_structure_refinement  'XL, SHELXTL v. 6.14 (Bruker, 2003)'
_computing_structure_solution    'Bruker (2006). APEX 2. Version 2.1.'
_diffrn_ambient_temperature      173(2)
_diffrn_detector_area_resol_mean 8.26
_diffrn_measured_fraction_theta_full 0.988
_diffrn_measured_fraction_theta_max 0.988
_diffrn_measurement_device_type
;
  Bruker-Nonius X8kappa APEX II CCD area detector'
;
_diffrn_measurement_method       'phi and omega scans with narrow frames'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0266
_diffrn_reflns_av_sigmaI/netI    0.0208
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            39873
_diffrn_reflns_theta_full        30.60
_diffrn_reflns_theta_max         30.60
_diffrn_reflns_theta_min         2.24
_diffrn_standards_decay_%        0
_exptl_absorpt_coefficient_mu    2.326
_exptl_absorpt_correction_T_max  0.6733
_exptl_absorpt_correction_T_min  0.6334
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
  SADABS, Bruker (2006). APEX 2. Version 2.1. Bruker Analytical
  X-ray Solutions, Madison, Wisconsin, USA.
;
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    2.550
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       prism
_exptl_crystal_F_000             810
_exptl_crystal_size_max          0.20
_exptl_crystal_size_mid          0.19
_exptl_crystal_size_min          0.17
_refine_diff_density_max         1.391
_refine_diff_density_min         -1.459
_refine_diff_density_rms         0.156
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.038
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     339
_refine_ls_number_reflns         6695
_refine_ls_number_restraints     127
_refine_ls_restrained_S_all      1.054
_refine_ls_R_factor_all          0.0402
_refine_ls_R_factor_gt           0.0330
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0490P)²+3.7461P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0883
_refine_ls_wR_factor_ref         0.0914
_reflns_number_gt                5639
_reflns_number_total             6695
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c4dt01733a2.cif
_cod_data_source_block           4
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Triclinic' changed to 'triclinic'
according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2281 2013-09-26 08:29:07Z andrius 

 Adding full bibliography for 7031708--7031711.cif.
;
_cod_original_cell_volume        1095.26(13)
_cod_database_code               7031711
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Mo1 Mo 0.12977(3) 0.22952(3) 0.32977(3) 0.01949(7) Uani 1 1 d U
Mo2 Mo 0.34362(3) 0.52440(3) 0.50062(3) 0.01493(7) Uani 1 1 d U
Mo3 Mo 0.34690(3) 0.49328(3) 0.21554(3) 0.01814(7) Uani 1 1 d U
Mo4 Mo 0.60153(3) 0.76344(3) 0.37342(3) 0.01850(7) Uani 1 1 d U
O1 O 0.0611(5) 0.1570(4) 0.1645(4) 0.0566(10) Uani 1 1 d U
O2 O 0.0159(3) 0.1420(3) 0.3814(3) 0.0310(6) Uani 1 1 d U
O3 O 0.2493(3) 0.3636(2) 0.5253(3) 0.0206(5) Uani 1 1 d U
O4 O 0.2641(3) 0.3978(2) 0.3158(3) 0.0192(5) Uani 1 1 d U
O5 O 0.2129(3) 0.6067(3) 0.4480(3) 0.0219(5) Uani 1 1 d U
O6 O 0.4657(3) 0.5992(2) 0.6703(3) 0.0193(5) Uani 1 1 d U
O7 O 0.4661(3) 0.5958(2) 0.4204(2) 0.0166(4) Uani 1 1 d U
O8 O 0.5129(3) 0.6253(3) 0.2240(3) 0.0209(5) Uani 1 1 d U
O9 O 0.3338(5) 0.4110(4) 0.0573(4) 0.0556(11) Uani 1 1 d U
O10 O 0.2514(6) 0.3322(5) 0.0909(4) 0.0636(12) Uani 1 1 d U
O11 O 0.2224(3) 0.5815(3) 0.1497(3) 0.0262(6) Uani 1 1 d U
O12 O 0.4605(3) 0.8394(3) 0.3280(3) 0.0250(5) Uani 1 1 d U
O13 O 0.7259(3) 0.8589(3) 0.3369(3) 0.0281(6) Uani 1 1 d U
O14 O 0.6948(3) 0.8268(2) 0.5676(3) 0.0217(5) Uani 1 1 d U
N1 N -0.0159(3) 0.3590(3) 0.2734(3) 0.0203(6) Uani 1 1 d U
N2 N -0.1387(4) 0.4927(4) 0.1650(4) 0.0278(7) Uani 1 1 d DU
H2N H -0.176(5) 0.538(4) 0.099(4) 0.033 Uiso 1 1 d D
C1 C -0.0521(4) 0.4186(4) 0.1665(4) 0.0239(7) Uani 1 1 d U
H1 H -0.0207 0.4095 0.1010 0.029 Uiso 1 1 calc R
C2 C -0.1609(5) 0.4805(4) 0.2747(4) 0.0291(8) Uani 1 1 d U
H2 H -0.2183 0.5222 0.2991 0.035 Uiso 1 1 calc R
C3 C -0.0844(4) 0.3968(4) 0.3414(4) 0.0250(7) Uani 1 1 d U
H3 H -0.0790 0.3690 0.4217 0.030 Uiso 1 1 calc R
O15 O 0.2012(9) 0.0321(8) 0.0347(9) 0.0493(19) Uani 0.50 1 d PD
H3OW H 0.232(11) 0.118(3) 0.059(12) 0.059 Uiso 0.50 1 d PD
H4OW H 0.106(4) 0.017(10) -0.026(10) 0.059 Uiso 0.50 1 d PD
O16 O 0.5123(4) 0.1070(3) 0.3747(4) 0.0387(8) Uani 1 1 d D
H1OW H 0.474(7) 0.021(2) 0.350(6) 0.053(18) Uiso 1 1 d D
H2OW H 0.444(4) 0.138(5) 0.383(5) 0.030(13) Uiso 1 1 d D
N3 N 0.5749(5) 0.1660(4) 0.1707(4) 0.0395(9) Uani 1 1 d DU
H3N H 0.548(6) 0.156(6) 0.234(5) 0.047 Uiso 1 1 d D
N4 N 0.6084(8) 0.2059(7) 0.0025(5) 0.087(2) Uani 1 1 d U
H4N H 0.6103 0.2387 -0.0666 0.105 Uiso 1 1 calc R
C4 C 0.5446(7) 0.2403(5) 0.0750(6) 0.0552(15) Uani 1 1 d U
H4 H 0.4903 0.3034 0.0606 0.066 Uiso 1 1 calc R
C5 C 0.6712(6) 0.1060(7) 0.0620(7) 0.0595(17) Uani 1 1 d U
H5 H 0.7198 0.0583 0.0313 0.071 Uiso 1 1 calc R
C6 C 0.6527(7) 0.0917(6) 0.1574(7) 0.0615(17) Uani 1 1 d U
H6 H 0.6902 0.0332 0.2168 0.074 Uiso 1 1 calc R
N5 N 0.8217(7) 0.1606(5) 0.6856(10) 0.080(2) Uani 1 1 d U
H5N H 0.7351 0.1605 0.6771 0.096 Uiso 1 1 calc R
N6 N 0.9882(7) 0.1486(4) 0.6419(7) 0.0588(14) Uani 1 1 d DU
H6N H 1.033(7) 0.142(7) 0.593(6) 0.071 Uiso 1 1 d D
C7 C 0.8475(10) 0.1380(6) 0.5869(7) 0.076(2) Uani 1 1 d U
H7 H 0.7779 0.1177 0.4928 0.091 Uiso 1 1 calc R
C8 C 1.0467(8) 0.1753(6) 0.7702(8) 0.0658(17) Uani 1 1 d U
H8 H 1.1481 0.1869 0.8323 0.079 Uiso 1 1 calc R
C9 C 0.9476(12) 0.1842(7) 0.8035(8) 0.075(2) Uani 1 1 d U
H9 H 0.9608 0.2034 0.8923 0.090 Uiso 1 1 calc R
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O2 Mo1 O1 104.41(18) . .
O2 Mo1 O14 100.14(13) . 2_666
O1 Mo1 O14 105.00(18) . 2_666
O2 Mo1 O4 156.43(13) . .
O1 Mo1 O4 94.48(16) . .
O14 Mo1 O4 88.19(10) 2_666 .
O2 Mo1 N1 86.36(13) . .
O1 Mo1 N1 93.52(18) . .
O14 Mo1 N1 157.97(11) 2_666 .
O4 Mo1 N1 78.41(11) . .
O2 Mo1 O3 90.42(13) . .
O1 Mo1 O3 164.69(16) . .
O14 Mo1 O3 75.49(10) 2_666 .
O4 Mo1 O3 70.21(10) . .
N1 Mo1 O3 83.50(10) . .
O5 Mo2 O6 104.04(12) . .
O5 Mo2 O3 103.74(12) . .
O6 Mo2 O3 100.74(12) . .
O5 Mo2 O7 103.43(11) . .
O6 Mo2 O7 98.41(11) . .
O3 Mo2 O7 141.60(11) . .
O5 Mo2 O4 98.53(11) . .
O6 Mo2 O4 157.29(11) . .
O3 Mo2 O4 76.01(11) . .
O7 Mo2 O4 73.55(10) . .
O5 Mo2 O7 179.37(11) . 2_666
O6 Mo2 O7 75.53(10) . 2_666
O3 Mo2 O7 75.92(9) . 2_666
O7 Mo2 O7 77.12(10) . 2_666
O4 Mo2 O7 81.93(9) . 2_666
O11 Mo3 O9 101.17(15) . .
O11 Mo3 O10 102.79(17) . .
O9 Mo3 O10 39.7(2) . .
O11 Mo3 O4 98.01(12) . .
O9 Mo3 O4 121.17(17) . .
O10 Mo3 O4 81.97(18) . .
O11 Mo3 O8 95.36(13) . .
O9 Mo3 O8 85.18(18) . .
O10 Mo3 O8 124.03(18) . .
O4 Mo3 O8 147.01(11) . .
O11 Mo3 O7 98.42(12) . .
O9 Mo3 O7 153.21(16) . .
O10 Mo3 O7 149.41(17) . .
O4 Mo3 O7 73.40(10) . .
O8 Mo3 O7 74.90(10) . .
O11 Mo3 O6 171.41(12) . 2_666
O9 Mo3 O6 85.71(13) . 2_666
O10 Mo3 O6 85.79(16) . 2_666
O4 Mo3 O6 82.54(10) . 2_666
O8 Mo3 O6 79.98(10) . 2_666
O7 Mo3 O6 73.47(9) . 2_666
O13 Mo4 O12 104.97(13) . .
O13 Mo4 O8 99.59(13) . .
O12 Mo4 O8 100.22(12) . .
O13 Mo4 O14 99.57(13) . .
O12 Mo4 O14 95.75(12) . .
O8 Mo4 O14 150.88(11) . .
O13 Mo4 O3 93.27(12) . 2_666
O12 Mo4 O3 160.49(12) . 2_666
O8 Mo4 O3 83.15(11) . 2_666
O14 Mo4 O3 74.05(10) . 2_666
O13 Mo4 O7 165.14(12) . .
O12 Mo4 O7 89.06(11) . .
O8 Mo4 O7 72.60(10) . .
O14 Mo4 O7 83.56(10) . .
O3 Mo4 O7 73.51(9) 2_666 .
Mo2 O3 Mo1 108.45(12) . .
Mo2 O3 Mo4 114.89(12) . 2_666
Mo1 O3 Mo4 93.02(10) . 2_666
Mo3 O4 Mo1 150.46(14) . .
Mo3 O4 Mo2 105.50(11) . .
Mo1 O4 Mo2 104.02(11) . .
Mo2 O6 Mo3 115.20(12) . 2_666
Mo2 O7 Mo3 103.86(11) . .
Mo2 O7 Mo4 153.46(13) . .
Mo3 O7 Mo4 93.95(9) . .
Mo2 O7 Mo2 102.88(10) . 2_666
Mo3 O7 Mo2 95.63(9) . 2_666
Mo4 O7 Mo2 94.63(9) . 2_666
Mo4 O8 Mo3 114.20(12) . .
O10 O9 Mo3 71.6(3) . .
O9 O10 Mo3 68.7(3) . .
Mo1 O14 Mo4 112.67(13) 2_666 .
C1 N1 C3 106.8(3) . .
C1 N1 Mo1 125.7(3) . .
C3 N1 Mo1 127.5(3) . .
C1 N2 C2 108.4(3) . .
C1 N2 H2N 122(3) . .
C2 N2 H2N 129(3) . .
N2 C1 N1 109.9(3) . .
N2 C1 H1 125.0 . .
N1 C1 H1 125.0 . .
C3 C2 N2 106.2(3) . .
C3 C2 H2 126.9 . .
N2 C2 H2 126.9 . .
C2 C3 N1 108.6(3) . .
C2 C3 H3 125.7 . .
N1 C3 H3 125.7 . .
H3OW O15 H4OW 105(3) . .
H1OW O16 H2OW 105(5) . .
C6 N3 C4 109.2(6) . .
C6 N3 H3N 118(4) . .
C4 N3 H3N 133(4) . .
C4 N4 C5 105.2(5) . .
C4 N4 H4N 127.4 . .
C5 N4 H4N 127.4 . .
N3 C4 N4 105.0(5) . .
N3 C4 H4 127.5 . .
N4 C4 H4 127.5 . .
C6 C5 N4 108.4(6) . .
C6 C5 H5 125.8 . .
N4 C5 H5 125.8 . .
C5 C6 N3 112.1(6) . .
C5 C6 H6 123.9 . .
N3 C6 H6 123.9 . .
C7 N5 C9 109.3(6) . .
C7 N5 H5N 125.3 . .
C9 N5 H5N 125.3 . .
C8 N6 C7 109.8(6) . .
C8 N6 H6N 127(5) . .
C7 N6 H6N 123(5) . .
N5 C7 N6 106.1(6) . .
N5 C7 H7 126.9 . .
N6 C7 H7 126.9 . .
N6 C8 C9 109.6(7) . .
N6 C8 H8 125.2 . .
C9 C8 H8 125.2 . .
C8 C9 N5 105.2(7) . .
C8 C9 H9 127.4 . .
N5 C9 H9 127.4 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Mo1 O2 1.709(3) .
Mo1 O1 1.720(4) .
Mo1 O14 1.930(3) 2_666
Mo1 O4 2.116(3) .
Mo1 N1 2.189(3) .
Mo1 O3 2.200(3) .
Mo2 O5 1.690(3) .
Mo2 O6 1.759(3) .
Mo2 O3 1.907(3) .
Mo2 O7 1.963(2) .
Mo2 O4 2.117(3) .
Mo2 O7 2.464(2) 2_666
Mo3 O11 1.696(3) .
Mo3 O9 1.879(4) .
Mo3 O10 1.914(4) .
Mo3 O4 1.942(3) .
Mo3 O8 1.978(3) .
Mo3 O7 2.141(2) .
Mo3 O6 2.277(3) 2_666
Mo4 O13 1.718(3) .
Mo4 O12 1.734(3) .
Mo4 O8 1.895(3) .
Mo4 O14 1.947(3) .
Mo4 O3 2.248(3) 2_666
Mo4 O7 2.304(2) .
O3 Mo4 2.248(2) 2_666
O6 Mo3 2.277(3) 2_666
O7 Mo2 2.464(2) 2_666
O9 O10 1.288(7) .
O14 Mo1 1.930(3) 2_666
N1 C1 1.329(5) .
N1 C3 1.372(5) .
N2 C1 1.328(5) .
N2 C2 1.372(5) .
N2 H2N 0.888(19) .
C1 H1 0.9500 .
C2 C3 1.355(6) .
C2 H2 0.9500 .
C3 H3 0.9500 .
O15 H3OW 0.89(2) .
O15 H4OW 0.89(2) .
O16 H1OW 0.90(2) .
O16 H2OW 0.897(19) .
N3 C6 1.308(8) .
N3 C4 1.334(7) .
N3 H3N 0.89(2) .
N4 C4 1.359(10) .
N4 C5 1.413(10) .
N4 H4N 0.8800 .
C4 H4 0.9500 .
C5 C6 1.192(10) .
C5 H5 0.9500 .
C6 H6 0.9500 .
N5 C7 1.285(11) .
N5 C9 1.341(11) .
N5 H5N 0.8800 .
N6 C8 1.270(9) .
N6 C7 1.303(10) .
N6 H6N 0.89(2) .
C7 H7 0.9500 .
C8 C9 1.290(11) .
C8 H8 0.9500 .
C9 H9 0.9500 .
loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
N4 H4N O8 0.88 2.43 3.144(8) 138.5 2_665
N6 H6N O2 0.89(2) 2.31(4) 3.087(6) 145(6) 1_655
N6 H6N O13 0.89(2) 2.30(6) 2.954(6) 130(6) 2_766
N3 H3N O16 0.89(2) 1.87(2) 2.747(6) 168(6) .
O16 H2OW O14 0.897(19) 1.90(2) 2.773(4) 165(5) 2_666
O16 H1OW O12 0.90(2) 1.91(3) 2.771(4) 161(6) 1_545
O15 H4OW O1 0.89(2) 2.19(8) 2.876(9) 134(9) 2
O15 H3OW O10 0.89(2) 2.25(4) 3.121(9) 166(9) .
O15 H3OW O1 0.89(2) 2.68(13) 2.961(8) 100(9) .
N2 H2N O10 0.888(19) 2.52(2) 3.407(6) 173(5) 2_565
N2 H2N O9 0.888(19) 1.99(3) 2.830(5) 156(5) 2_565
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O5 Mo2 O3 Mo1 86.57(14) . .
O6 Mo2 O3 Mo1 -165.94(11) . .
O7 Mo2 O3 Mo1 -47.3(2) . .
O4 Mo2 O3 Mo1 -8.96(10) . .
O7 Mo2 O3 Mo1 -93.98(11) 2_666 .
O5 Mo2 O3 Mo4 -170.95(13) . 2_666
O6 Mo2 O3 Mo4 -63.46(15) . 2_666
O7 Mo2 O3 Mo4 55.2(2) . 2_666
O4 Mo2 O3 Mo4 93.52(13) . 2_666
O7 Mo2 O3 Mo4 8.49(11) 2_666 2_666
O2 Mo1 O3 Mo2 -157.03(14) . .
O1 Mo1 O3 Mo2 8.7(7) . .
O14 Mo1 O3 Mo2 102.60(14) 2_666 .
O4 Mo1 O3 Mo2 9.24(10) . .
N1 Mo1 O3 Mo2 -70.74(13) . .
O2 Mo1 O3 Mo4 85.45(12) . 2_666
O1 Mo1 O3 Mo4 -108.8(6) . 2_666
O14 Mo1 O3 Mo4 -14.92(10) 2_666 2_666
O4 Mo1 O3 Mo4 -108.27(11) . 2_666
N1 Mo1 O3 Mo4 171.74(11) . 2_666
O11 Mo3 O4 Mo1 95.9(3) . .
O9 Mo3 O4 Mo1 -12.4(3) . .
O10 Mo3 O4 Mo1 -6.0(3) . .
O8 Mo3 O4 Mo1 -151.1(2) . .
O7 Mo3 O4 Mo1 -167.6(3) . .
O6 Mo3 O4 Mo1 -92.7(3) 2_666 .
O11 Mo3 O4 Mo2 -82.22(13) . .
O9 Mo3 O4 Mo2 169.50(15) . .
O10 Mo3 O4 Mo2 175.90(17) . .
O8 Mo3 O4 Mo2 30.7(2) . .
O7 Mo3 O4 Mo2 14.23(10) . .
O6 Mo3 O4 Mo2 89.13(11) 2_666 .
O2 Mo1 O4 Mo3 -149.9(3) . .
O1 Mo1 O4 Mo3 -6.4(3) . .
O14 Mo1 O4 Mo3 98.5(3) 2_666 .
N1 Mo1 O4 Mo3 -99.1(3) . .
O3 Mo1 O4 Mo3 173.7(3) . .
O2 Mo1 O4 Mo2 28.3(3) . .
O1 Mo1 O4 Mo2 171.73(18) . .
O14 Mo1 O4 Mo2 -83.36(12) 2_666 .
N1 Mo1 O4 Mo2 79.05(12) . .
O3 Mo1 O4 Mo2 -8.13(9) . .
O5 Mo2 O4 Mo3 86.03(13) . .
O6 Mo2 O4 Mo3 -87.5(3) . .
O3 Mo2 O4 Mo3 -171.84(14) . .
O7 Mo2 O4 Mo3 -15.54(10) . .
O7 Mo2 O4 Mo3 -94.42(11) 2_666 .
O5 Mo2 O4 Mo1 -93.02(12) . .
O6 Mo2 O4 Mo1 93.5(3) . .
O3 Mo2 O4 Mo1 9.11(10) . .
O7 Mo2 O4 Mo1 165.41(13) . .
O7 Mo2 O4 Mo1 86.53(10) 2_666 .
O5 Mo2 O6 Mo3 176.14(13) . 2_666
O3 Mo2 O6 Mo3 68.88(14) . 2_666
O7 Mo2 O6 Mo3 -77.66(13) . 2_666
O4 Mo2 O6 Mo3 -10.5(4) . 2_666
O7 Mo2 O6 Mo3 -3.38(10) 2_666 2_666
O5 Mo2 O7 Mo3 -81.12(13) . .
O6 Mo2 O7 Mo3 172.18(11) . .
O3 Mo2 O7 Mo3 52.9(2) . .
O4 Mo2 O7 Mo3 13.95(9) . .
O7 Mo2 O7 Mo3 99.21(12) 2_666 .
O5 Mo2 O7 Mo4 49.6(3) . .
O6 Mo2 O7 Mo4 -57.1(3) . .
O3 Mo2 O7 Mo4 -176.4(2) . .
O4 Mo2 O7 Mo4 144.7(3) . .
O7 Mo2 O7 Mo4 -130.0(3) 2_666 .
O5 Mo2 O7 Mo2 179.67(11) . 2_666
O6 Mo2 O7 Mo2 72.97(11) . 2_666
O3 Mo2 O7 Mo2 -46.4(2) . 2_666
O4 Mo2 O7 Mo2 -85.25(10) . 2_666
O7 Mo2 O7 Mo2 0.0 2_666 2_666
O11 Mo3 O7 Mo2 80.65(14) . .
O9 Mo3 O7 Mo2 -142.7(3) . .
O10 Mo3 O7 Mo2 -53.0(4) . .
O4 Mo3 O7 Mo2 -15.25(10) . .
O8 Mo3 O7 Mo2 173.97(13) . .
O6 Mo3 O7 Mo2 -102.23(12) 2_666 .
O11 Mo3 O7 Mo4 -79.51(12) . .
O9 Mo3 O7 Mo4 57.1(3) . .
O10 Mo3 O7 Mo4 146.9(3) . .
O4 Mo3 O7 Mo4 -175.42(11) . .
O8 Mo3 O7 Mo4 13.81(9) . .
O6 Mo3 O7 Mo4 97.61(10) 2_666 .
O11 Mo3 O7 Mo2 -174.57(11) . 2_666
O9 Mo3 O7 Mo2 -37.9(3) . 2_666
O10 Mo3 O7 Mo2 51.8(3) . 2_666
O4 Mo3 O7 Mo2 89.52(10) . 2_666
O8 Mo3 O7 Mo2 -81.25(10) . 2_666
O6 Mo3 O7 Mo2 2.55(8) 2_666 2_666
O13 Mo4 O7 Mo2 152.9(4) . .
O12 Mo4 O7 Mo2 -46.1(3) . .
O8 Mo4 O7 Mo2 -147.1(3) . .
O14 Mo4 O7 Mo2 49.8(3) . .
O3 Mo4 O7 Mo2 125.0(3) 2_666 .
O13 Mo4 O7 Mo3 -74.6(5) . .
O12 Mo4 O7 Mo3 86.42(12) . .
O8 Mo4 O7 Mo3 -14.59(10) . .
O14 Mo4 O7 Mo3 -177.68(11) . .
O3 Mo4 O7 Mo3 -102.44(10) 2_666 .
O13 Mo4 O7 Mo2 21.4(5) . 2_666
O12 Mo4 O7 Mo2 -177.59(11) . 2_666
O8 Mo4 O7 Mo2 81.39(10) . 2_666
O14 Mo4 O7 Mo2 -81.69(10) . 2_666
O3 Mo4 O7 Mo2 -6.46(8) 2_666 2_666
O13 Mo4 O8 Mo3 -175.65(14) . .
O12 Mo4 O8 Mo3 -68.40(16) . .
O14 Mo4 O8 Mo3 53.8(3) . .
O3 Mo4 O8 Mo3 92.17(13) 2_666 .
O7 Mo4 O8 Mo3 17.36(11) . .
O11 Mo3 O8 Mo4 78.79(15) . .
O9 Mo3 O8 Mo4 179.58(17) . .
O10 Mo3 O8 Mo4 -171.84(18) . .
O4 Mo3 O8 Mo4 -34.9(3) . .
O7 Mo3 O8 Mo4 -18.50(12) . .
O6 Mo3 O8 Mo4 -93.93(13) 2_666 .
O11 Mo3 O9 O10 -96.6(3) . .
O4 Mo3 O9 O10 10.0(3) . .
O8 Mo3 O9 O10 168.8(3) . .
O7 Mo3 O9 O10 127.2(4) . .
O6 Mo3 O9 O10 88.6(3) 2_666 .
O11 Mo3 O10 O9 92.1(3) . .
O4 Mo3 O10 O9 -171.4(3) . .
O8 Mo3 O10 O9 -13.5(3) . .
O7 Mo3 O10 O9 -135.1(3) . .
O6 Mo3 O10 O9 -88.4(3) 2_666 .
O13 Mo4 O14 Mo1 -72.21(16) . 2_666
O12 Mo4 O14 Mo1 -178.48(14) . 2_666
O8 Mo4 O14 Mo1 58.3(3) . 2_666
O3 Mo4 O14 Mo1 18.48(12) 2_666 2_666
O7 Mo4 O14 Mo1 93.12(13) . 2_666
O2 Mo1 N1 C1 -143.9(3) . .
O1 Mo1 N1 C1 -39.6(3) . .
O14 Mo1 N1 C1 107.9(4) 2_666 .
O4 Mo1 N1 C1 54.2(3) . .
O3 Mo1 N1 C1 125.3(3) . .
O2 Mo1 N1 C3 37.8(3) . .
O1 Mo1 N1 C3 142.0(3) . .
O14 Mo1 N1 C3 -70.5(5) 2_666 .
O4 Mo1 N1 C3 -124.1(3) . .
O3 Mo1 N1 C3 -53.1(3) . .
C2 N2 C1 N1 -0.4(5) . .
C3 N1 C1 N2 0.5(4) . .
Mo1 N1 C1 N2 -178.1(3) . .
C1 N2 C2 C3 0.1(5) . .
N2 C2 C3 N1 0.2(5) . .
C1 N1 C3 C2 -0.5(4) . .
Mo1 N1 C3 C2 178.1(3) . .
C6 N3 C4 N4 0.3(6) . .
C5 N4 C4 N3 1.7(6) . .
C4 N4 C5 C6 -3.3(7) . .
N4 C5 C6 N3 3.7(7) . .
C4 N3 C6 C5 -2.6(7) . .
C9 N5 C7 N6 -0.6(7) . .
C8 N6 C7 N5 0.7(7) . .
C7 N6 C8 C9 -0.6(8) . .
N6 C8 C9 N5 0.2(8) . .
C7 N5 C9 C8 0.3(7) . .
